Summary of silk-producing glands, fiber types and silk proteins found in the threads of orb- or cob-weavers. (*Only identified in orb-weaver’s spiral capture silk)
In the past few years a number of reviews, books and journal articles featuring silks have been published. Silks are produced by over 41,000 species of spiders (class Arachnida) and by many insects (terrestrial and aquatic), particularly in the order Lepidoptera (Foelix, 1996); they are defined as externally spun fibrous material generated from protein secretions. The cocoon silk from the domesticated silkmoth,
2. Diversity of spider silks
As scientists unravel the secrets of spider silk, it has become evident that a broad range of diverse fiber types has evolved to serve different ecological purposes. These threads have a host of different functions: locomotion, wrapping prey, protection of developing eggs and web construction. The structural diversity of spider silk fibers can be attributed to over 400 million years of natural selection. Anatomical studies of typical orb or cob-weavers reveal the presence of seven distinct silk-producing glands: the major and minor ampullate glands (locomotion and web frame), tubuliform (egg case silk), flagelliform (spiral capture silk), aciniform (prey wrapping silk), aggregate (sticky adhesives on spiral capture or gumfooted lines), and the pyriform glands (attachment disc and joining fibers) (Fig. 1). Molecular and biochemical analyses demonstrate that the different silk-producing glands are highly specialized, expressing specific members of the spider silk gene superfamily (Table 1). Through the evolution of different silk-producing glands, spiders can express gland-specific silk proteins with different sequences, generating a broad range of different fiber types with diverse functional attributes (Guerette et al., 1996).
2.1. Major ampullate silks
The major ampullate gland has been the principal focus for researchers investigating the natural silk production pathway. This bulb-shaped gland is found in pairs in spiders and is responsible for producing dragline silk (Fig. 1). Dragline silk is referred to as the ‘safety line’ of spiders and it is often spun in pairs and is accompanied with two minor ampullate silk threads (Fig. 2A). During locomotion, dragline silk fibers are immobilized to surfaces by structures known as attachment discs. Attachment discs are comprised of small diameter fibers spun from the pyriform gland that are extruded in a sticky substance that dries rapidly, sealing dragline silk to wood, concrete, glass, plants and other materials (Fig. 2B). The mechanical properties of major ampullate silk are dependent upon the amino acid sequences of the spun fibroins and the reeling speed during extrusion. When major ampullate silks are spun rapidly, it produces a stiffer fiber that efficiently supports the weight of spiders. In contrast, spinning major ampullate silk at a slower rate during the web frame construction leads to a fiber with higher extensibility, a necessity for dissipating the energy of prey impact on the web. Transmission electron microscopic analysis reveals dragline silk contains four different layers: core, skin, glycoprotein layer and a lipid coat (Sponner et al., 2007). These studies also demonstrate that dragline silk threads lack adhesive coatings on their surface.
|Silk Gland||Location of Silk||Fiber Proteins|
|Major ampullate||Web frame, safety line (dragline)||MaSp1; MaSp2|
|Minor ampullate||Web reinforcement , safety line (dragline)||MiSp1-like|
|Flagelliform||Spiral capture silk*||Flag*|
|Aciniform||Wrapping silk, small diameter egg case fiber||AcSp1-like|
|Tubuliform||Large diameter egg case fiber||TuSp1; ECP-1; ECP-2|
|Aggregate||Glue coating for gumfooted lines||Unknown|
|Pyriform||Attachment disk and joining fiber||PySp1|
In orb-weaving spiders the functions for dragline silk include web frame construction and locomotion. Black widow spiders also use dragline silk to build three-dimensional webs for prey capture. We have shown by MS/MS analyses that solubilized proteins from scaffolding, gumfooted and dragline silk fibers, followed by tryptic digestion, produce overlapping peptide fingerprints that match protein sequences within the major ampullate fibroins (unpublished data). These studies demonstrate scaffolding, gumfooted lines and dragline silk consists of major ampullate silks. Because scaffolding silk fibers represent the bulk of a black widow spider’s three-dimensional web, it provides an excellent opportunity to collect dragline silk from black widow spiders housed in cages. The collection of large amounts of scaffolding silk can be done rapidly from spiders stored within the laboratory. Milligram quantities can be obtained from a single cage that is 1’ x 1’ x 1.5’. In order to produce regenerated major ampullate silk, we have taken advantage of the fact that scaffolding fibers are a rich source of full-length protein sequences for the major ampullate silk fibroins.
2.2. Egg sac silks
Of the seven different silk types spun from spiders, egg case silks are the easiest to collect. When egg sacs are spun from female spiders, they must endure a variety of different environmental factors. Some of these factors include predators and invasion by parasites or temperature and humidity fluctuations. Black widow spider egg sacs contain two thread types: aciniform and tubuliform silks (Fig. 2C-D). Aciniform fibers have diameter sizes that are approximately 500 nm, which is one order of magnitude smaller than the average 5 μm diameter sizes for tubuliform silks. These fibers are also coated with small droplets, but the chemical contents of the liquid material have not been determined (Fig. 2C-D). In addition to the structural proteins in the fibers, MS/MS analysis has identified the presence of two spider coating peptides, which have been named SCP-1 and SCP-2. Intriguingly, these peptides can be efficiently removed from egg sacs soaked in water, suggesting these peptides are water soluble, polar compounds (Hu et al., 2007). The biological significance of the coating peptides is presently unknown, but one hypothesis is these molecules function as antimicrobial agents that help prolong the longevity of the fibers. Quantitative real-time PCR analysis has demonstrated that SCP mRNA levels are elevated in the flagelliform gland (Blasingame et al., 2009).
In addition to aciniform silks being constituents of egg cases, these fibers are also used for prey capture (Hayashi et al., 2004; Vasanthavada et al., 2007). Because detailed molecular data are available for dragline and tubuliform silks and these fiber types are available in large quantities, we are attempting to study the mechanical behavior of synthetic composite spider silk threads spun from regenerated dragline and egg sac silk protein mixtures. Additionally, we are supplementing regenerated dragline silk fibroins with different recombinantly expressed spider silk proteins. This approach has many advantages, including the ability to have native-sized full-length fibroins in artificially spun fibers with truncated recombinant proteins.
3. Properties and compositions of spider silk
Spider silks represent natural composite materials that are biopolymers. Biochemical analyses reveal that the different silk types contain at least 2-3 distinct structural proteins, commonly referred to as fibroins. Table 1 summarizes the major proteins stored within the luminal contents of several silk-producing glands within
3.1. Molecular components of dragline silk
The major and minor ampullate fibroins contain the highest levels of glycine and alanine relative to other spider silk family members; these levels approach >50% of the total amino acid content (Casem et al., 1999; Lombardi & Kaplan, 1990). Biochemical experiments show dragline silk is a composite material largely composed of two structural proteins or spidroins (contraction of the words spider and fibroin) called MaSp1 and MaSp2 (Xu and Lewis, 1990; Hinman and Lewis, 1992). Structural studies demonstrate the major ampullate spidroins form the core of the fiber that is wrapped inside a glycoprotein coat. Although the identities of the constituents of the glycoprotein layer remain unknown, experimental evidence supports this layer is added in the ampulla prior to extrusion (Casem et al., 2002; Sponner et al., 2005). The molecular sequences coding for the dragline silk fibroins were the first to be identified from
3.2. Molecular components of tubuliform silks
Tubuliform fibroins have been shown to contain considerably lower levels of glycine relative to dragline silk. Similar to pyriform silks, tubuliform silks incorporate amino acids with more polar side chain groups (Blasingame et al., 2009). Although dragline silk fibers have received much attention in the scientific community, the molecular and structural details for egg case silk fibers are rapidly emerging. Egg sacs are produced by female spiders during reproductive periods. For black widow spiders, egg cases are composite materials containing two different silk types: tubuliform and aciniform (Vasanthavada et al., 2007). The presence of two different fiber types implies tubuliform and aciniform fibers provide a unique role that is central to the protection of spiderlings during development. Biochemical studies have shown that aciniform silks contain the fibroin AcSp1-like (Vasanthavada et al., 2007) and the tubuliform silks contain at least three different proteins: TuSp1, ECP-1 and ECP-2 (Hu et al., 2005; 2006b). Scanning electron microscopy, along with amino acid composition analyses performed on the egg sacs, support that tubuliform silks, based upon volume, constitute the bulk of egg sac fibers. Additionally, mass spectrometry studies (MS/MS) demonstrate that TuSp1 is one of the major constituents of tubuliform silks and the non-repetitive N-terminus is retained in the spun fibroin. Manual inspection of the amino acid sequence of TuSp1 reveals high levels of serine and alanine, but lower levels of glycine. This fibroin lacks the traditional An, (GA)n, (GGX)n and (GPGXX)n repeats, but it contains new amino acid motifs that include Sn, (SA)n, (SQ)n, and GX (X represents A, D, F, I, N, Q, V and Y). Internal block repeats are ~184 amino acids in length and are extremely homogenous in nature. Short polyalanine stretches are highly iterated in the TuSp1 sequence and 13C NMR spectroscopy demonstrates that the majority of alanine is in a beta-sheet structure in post-spun egg case silk (Hu et al., 2005).
The ECPs (ECP-1 and ECP-2) are also components of tubuliform silks (Hu et al., 2006b). Based on Q-PCR studies, TuSp1 mRNA levels are ~20-fold higher relative to the ECPs. Both ECP-1 and ECP-2 contain large amounts of alanine, glycine and serine. These residues account for more than 50% of all of the amino acids in their translated sequences. Translation of the ECP-1 and ECP-2 cDNAs predict proteins with 932 and 825 amino acids, respectively. The N-terminal 182 residues of ECP-1 and ECP-2 are 70% identical, with 16 cysteine residues showing identical spacing patterns and 100% conservation. Whether these cysteines participate in disulfide bond formation with each other or the N-termini of TuSp1, which has two cysteine residues within its non-repetitive conserved terminus, is unknown. The ECPs lack traditional internal block repeats commonly found in spidroin family members, however, ECP-2 contains scattered, internal blocks of polyalanine and a C-terminus rich in GA repeats. To date, the orb-weaver ECP orthologues have not been reported. The precise role the ECPs serve in tubuliform silks is unclear, but their rich alanine and glycine content, similar to dragline silk fibroins, suggests structural importance.
4. Mechanical properties of spider silk
The mechanical properties of spider silks have been shown to be highly renowned relative to some of the best man-made materials, displaying a combination of high strength, extensibility and toughness. With respect to energy absorption prior to breaking, spider silks are unmatched in the world of synthetic and natural fibers (Table 2). Different spider silk types produce distinct stress-strain curves, demonstrating that spiders spin a broad range of fibers with diverse mechanical properties (Gosline et al., 1986; Hu et al., 2006a). Similar to other protein polymers, there are numerous factors that influence the strength and the load-deformation response of silk fibers, which includes temperature, humidity, and extrusion rate. The majority of mechanical studies have focused on dragline silk. Dragline silk fibers have been subject to tensile testing from a wide range of different spider species. Natural dragline silk fibers show both extremely high tensile strength and toughness (often measured as “Energy to Break”). In man-made polymers, such as polyethylene, increasing strength would often compromise fracture toughness. Yet in the dragline silk, both strength and toughness can be maintained at high levels. The variations in the mechanical behavior in dragline silk fibers across different species suggest that these silks have been fine-tuned by each spider for their nuanced needs. Other spider silk fiber types have also been studied using tensile testing, including aciniform silks (Hayashi et al., 2004), tubuliform silks (Hu et al., 2006a), flagelliform silks (Lewis, 2006) and minor ampullate silks (Liivak et al., 1997).
|Fiber||Elongation (%)||Strength (GPa)||Energy to Break (MJ/m3)|
|Kevlar 49 fiber||2.7||3.6||50|
4.1. Dragline silk
Dragline silk is five times stronger by weight than steel and three times tougher than the man-made fiber Kevlar, a synthetic fiber used in body armor (Table 2). Correlations between the reeling speed and the tensile strength of dragline silk fibers have been observed experimentally, supporting that spiders can tailor their thread properties by adjusting the draw rate from their spinnerets. By controlling the reeling speeds during extrusion, spiders can tune beta-sheet crystallite size and orientation of the protein polypeptide chain network. These parameters are important structural factors that modulate the tensile strength of silks (Du et al., 2006). Studies investigating the effects of reeling speeds demonstrate 3 nm nanocrystals are optimal for producing fibers that have exceptionally high tensile strength.
Consistent with this observation, molecular modeling stress-strain simulations predict that 3 nm crystals, which correlate to the natural size found in dragline silk, have higher ultimate strengths and toughness relative to fibers with larger nanocrystal sizes (Nova et al., 2010). This implies that spiders can manipulate the material properties of their fibers by changing the reeling speed to tune the size of the beta-sheet nanocrystals.
Spider dragline silk fibers have been shown to be thermally stable to about 2300C on thermal gravimetric analysis. In addition, these fibers have been shown to be able retain their morphology, structure and mechanical properties when autoclaved (Hedhammar et al., 2010). Unlike tubuliform silks, natural dragline silk fibers have been shown to experience supercontraction when exposed to water, resulting in shrinking by up to 50% in length. For certain silk types, supercontraction may provide an important mechanism to tailor silk properties for synthetic composite spider silks.
4.2. Minor, aciniform and flagelliform silk
Similar to major ampullate silks, minor ampullate silks have been shown to display a high Young’s modulus (Liivak et al., 1997). In addition, mechanical studies have demonstrated that aciniform silks represent the toughest spider silk type (Hayashi et al., 2004), a likely evolutionary adaptation to help prevent the escape of immobilized prey (Table 2). Previous biochemical analyses performed by our laboratory have demonstrated that aciniform silks are also constituents of egg case silk in black widow spiders. The presence of aciniform silks in egg sacs is intriguing, but it may suggest these fibers function to prevent predators from gaining access to the enclosed eggs. Flagelliform silks, which have only been studied from orb-weavers, are highly extensible fibers that constitute spiral capture silk (Lewis, 2006). Spiral capture silk fibers are strategically positioned in orb webs to absorb and dissipate large amounts of mechanical energy introduced during the collision of aerial insects (Lin et al., 1995). These fibers are extremely compliant, which results in energy dissipation through thread displacement and stretching (Table 2). Whether a functional equivalent of spiral capture silk fibers is present in black widow spiders is unclear. Black widow spiders cast three-dimensional webs, instead of two-dimensional webs that are characteristic of orb weavers. Therefore, it would appear that black widow spiders have replaced FLAG silk, which comprises the spiral capture silk fibers, with scaffolding silk or dragline silk. This observation supports that spiders have evolved specialized silk fibers and different web types to optimize prey capture.
4.3. Tubuliform silks
Tubuliform silks have been shown to be highly extensible, but display lower tensile breaking strength relative to dragline silk fibers (Hu et al. 2006a; Zhao et al., 2006). However, because tubuliform silks have increased extensibility relative to dragline silks, tubuliform fibers display similar toughness (Table 2). To our knowledge, no experiments have been reported to examine the mechanical properties of regenerated tubuliform silk.
5. Natural extrusion of silk
Many laboratories have focused on studying the extrusion process of dragline silk from the major ampullate gland, primarily because this tissue is the easiest to identify and remove. This structure is also the largest relative to the other silk-producing glands. Morphological and histological studies demonstrate the major ampullate gland consists of various components: it has a tail, ampulla, funnel and extrusion duct (Fig. 3).
Large quantities of major ampullate spidroins are manufactured from columnar epithelial cells residing in the tail, transported to the ampulla through vesicles, followed by extrusion through a duct that tapers down, finally exiting from a spigot positioned on an abdominal spinneret. In our microdissections of spiders, we also observe the presence of a small ampullate gland (SAG) that is connected to the major ampullate gland (Fig. 3) (Ortiz et al., 2000). The SAG is distinct from the minor ampullate gland (not shown) and it has received little attention in scientific literature. Intriguingly, the SAG has its own tail, ampulla, funnel and spinning duct that is fused to the extrusion duct of the major ampullate gland (Fig. 3). The specific biological function of the SAG or the molecular contents it synthesizes, stores and spins is unclear.
5.1. Biochemical processes during silk extrusion
To be able to produce synthetic spider silk composite fibers, scientists must first understand the natural spinning process. Biophysical studies of the liquid contents stored within the major ampulla, also referred to as the spinning dope, reveal these proteins are unfolded and have a disordered secondary structure (Knight et al., 2000; Lefevre et al., 2008). The spinning dope has been shown to represent a highly concentrated aqueous mixture of major ampullate spidroins. During extrusion, these spidroins undergo changes that alter their conformation and orientation. This process, which involves converting native liquid silk into insoluble fibers, is modulated by chemical and mechanical events (Fig. 4).
These events include changes in pH, salt concentration and elongational flow (Chen et al., 2002; Dicko et al. 2004; Knight & Vollrath, 2001). This course of action gives rise to a hierarchically organized semicrystalline material. The crystalline region consists of short polyalanine segments that form beta-sheet nanocrystals, whereas the amorphous phase is formed from glycine-rich segments that likely adopt 31-helices and a few alpha helices.
Histological data reveal that H+ pump activity increases steadily along the length of the spinning duct (Vollrath et al., 1998). Studies using a pH-sensitive microelectrode probe support this observation, demonstrating the pH decreases from 7.2 in the major ampullate gland to 6.3 in the extrusion duct (Dicko et al., 2004). Other chemical changes have been implicated in the transition from liquid to solid during fiber production. These include a decrease in Na+ ions, coupled with increased K+ and phosphate ion concentrations during extrusion (Huemmerich et al., 2004) (Fig. 3). The pH decrease in the extrusion duct has been associated with changes in the ionization state of side chain residues positioned within the conserved N- and C-termini of spidroins, promoting dimerization and fiber polymerization. Although the N- and C-termini both contain conserved non-repetitive regions, their amino acid sequences are dissimilar. However, despite the differences in amino acid sequences, there are some similarities in their conformational flexibility and secondary structures. Recent structural studies of the MaSp1 N-terminal domain (NT) from the nursery web spider,
The mechanisms of fiber extrusion in the other silk-producing glands have not been thoroughly investigated at the biochemical level. Analyses of the morphological features of these silk-producing glands reveal profound structural differences, aside from the architecture of the minor ampullate gland, which closely resembles the major ampullate gland (Jeffery et al., 2011). These data imply that the mechanisms for fiber extrusion are distinct in the different glands that produce silk. Raman spectroscopy studies performed on the glandular contents of the tubuliform gland support this supposition, which demonstrate proteins are stored in a globular conformation with a high degree of alpha helical nature; this differs significantly from the conformations of fibroins stored within the major ampullate gland (Lefevre et al., 2011). However, after spinning, the tubuliform silks are structurally similar to major ampullate fibers, containing a high degree of beta-sheet structure. NMR studies have been performed to analyze the secondary and tertiary structures of
6. Synthetic composite spider fibers from recombinant proteins
Although it is feasible to harvest milligrams of natural dragline silk by forcibly “milking” spiders or retrieving large amounts of tubuliform silks through the collection of egg sacs, these are expensive and time-consuming endeavors. For example, a 3.4 m textile weaved from natural dragline silk took more than one million
6.1. Silk fibroin expression
Both prokaryotic and eukaryotic expression systems have their advantages and disadvantages. For example, many eukaryotic proteins require posttranslational modifications for functional activity, such as glycosylation and phosphorylation. Although the significance of posttranslational modifications (PTMs) to fibroins remains unclear, amino acid residues have been shown to be subject to phosphorylation and glycosylation within fibroin sequences (Michal et al., 1996). Because PTMs are largely restricted to eukaryotic cells, expression systems equipped with the cellular machinery for PTMs offer benefits to potentially achieving fibroin states that resemble
6.2. Artificial fiber production
Despite the broad range of expression systems used to synthesize recombinant spider silk proteins, only a handful of research groups have spun artificial silk fibers using the recombinant spidroins (Geurts et al., 2010; Lazaris et al., 2002; Teule et al., 2009). Even fewer research labs have subsequently used these synthetic fibers to compare their mechanical properties to the natural fibers (Xia et al., 2010). For most labs that have participated in the production of recombinant silk fibroins, strategies have included using several block repeats and/or the non-repetitive C-terminal domain for expression studies. The majority of these studies have used either the major ampullate spidroin 1 or 2 (MaSp1 or MaSp2).
6.2.1. Composite silk fibers spun from regenerated major ampullate silk spidroins blended with recombinant proteins
Although synthetic silk fibers have been spun from recombinant spider silk proteins, silk filaments have also been reported from dissolving natural dragline silk and re-spinning the solubilized fibroin extract, a process that leads to a material known as regenerated silk. Regenerated dragline spider silk has been described in the scientific literature just a few times. These experiments have demonstrated reconstituted dragline spider silk self-assembles into filaments from
In our attempt to enhance the properties of regenerated dragline spider silk, we have supplemented this silk with recombinantly expressed truncated dragline silk fibroins, MaSp1 and MaSp2. These truncated forms, referred to as 1RCTMaSp1 and 1RCTMaSp2, consisted of one block repeat fused to the non-repetitive, conserved C-terminus. To facilitate recombinant protein solubility during induction in
In addition to morphological differences, the fibers of varying formulations also exhibit markedly different mechanical behavior. When compared with the native dragline, the regenerated dragline silk has reduced modulus, extensibility, and toughness (Fig. 6). Supplementing the regenerated dragline silk with either recombinant 1RCTMaSp1 or 1RCTMaSp2 increases the elastic modulus, tensile strength, and toughness over the regenerated dragline silk alone. However, supplementing with both recombinant 1RCTMaSp1 and 1RCTMaSp2 appears to diminish the mechanical enhancements relative to either fibroin alone, suggesting that specific combinations of fibroins may provide optimal mechanical behavior. The molecular basis is currently being investigated. Taken together, our synthetic composite dragline silk fibers display higher tensile strength and extensibility relative to previous reports involving artificial fibers spun from truncated recombinant MaSp1 and MaSp2 lacking their C-termini (Brooks et al. 2008). This supports that the C-terminus contributes to enhancing the mechanical properties of the blended fibers.
6.2.2. Composite silk fibers spun from regenerated aciniform and tubuliform silk proteins
Regenerated spider silk fibers spun from reconstituted egg sacs have not been reported in the scientific literature. Here we demonstrate that solubilization of black widow egg sacs with HFIP, followed by wet-spinning of the fibers into an isopropanol coagulation bath, can lead to a composite filament containing the fibroins AcSp1-like, TuSp1 and the ECP silk proteins. These artificial spider silk composites were spun from 20% (w/v) solutions of dissolved egg sacs. These are the first reported composite silk fibers that include native sized aciniform and tubuliform silk proteins blended together into a single filament. SEM studies demonstrated that the reconstituted egg case fibers contained diameter sizes approximately 90 μm (Fig. 7A). Analysis of the surface morphology of the fibers revealed more irregularities relative to the natural tubuliform silks (Compare Fig. 2D with 7A). The interior of fractured regenerated egg case fibers showed a solid core, suggesting that fibroin assembly was not impaired during the spinning process (Fig. 7B). Stress-strain curves performed on individual threads demonstrated these composite fibers were 2-fold lower and an order of magnitude below the tensile strength of natural tubuliform silk (Fig. 7C). The % strain and tensile strength was 30% and 83 MPa, respectively. In the future, we plan on testing the biocompatibility of these fibers to determine their suitability for applications, such as tissue engineering.
7. Other applications
Methodologies to spin artificial silk fibers on a large-scale for industrial, medical, military and commercial use are progressing rapidly. In addition to spinning silk threads for a host of applications other uses for spider silk proteins are being pursued, including drug delivery and scaffolding materials. Both dragline silk fibers and egg sacs have been studied for their biocompatibility in a few human cell culture systems (Allmeling et al., 2006; Gellynck et al., 2008). Primary chondrocytes have been shown to attach and survive for several weeks on natural dragline silk and egg sacs (Gellynck et al., 2008). Natural dragline silk fibers have also been used to culture human primary Schwann cells and demonstrate these cells can adhere and elongate (Allmeling et al., 2006).
Thus far, few
This chapter highlights how regenerated dragline and tubuliform silk fibroins can be used to generate a spinning dope suitable for synthetic fiber production. It also explores the use of blending truncated recombinantly expressed dragline silk fibroins MaSp1 and MaSp2 with reconstituted dragline silk fibroins to generate composite spider silk fibers. With the identification of different spider silk cDNAs, coupled with the advancements in heterologous protein expression systems and the spinning process, the timing to explore the production of new engineering materials that integrate different mixtures of recombinant silk proteins and reconstituted silk proteins provides an exciting time for silk biology research. We have taken a novel approach, combining regenerated silk fibroins with recombinant proteins, to study the material properties of synthetic composite spider silk fibers. Our studies demonstrate that infusion of recombinant proteins into solubilized regenerated silk fibroin mixtures is a valid method to study fibroin function in spun composite silk fibers. It is also a method to generate a vast number of diverse synthetic composite fibers with a broad range of mechanical functions.
We thank Anne Moore for the donation of her tensometer for the mechanical studies. In addition, we thank Kaitlen Colafrancesco and Coby La Mattina for their critical comments on the book chapter. We also are indebted to Dr. Mark Brunell at the University of the Pacific, Department of Biology, for his assistance with the scanning electron microscope. This work was supported by a NSF RUI Grant MCB-0950372 entitled Molecular Characterization of Black Widow Spider Silks.
Agapov I. Pustovalova O. L. Moisenovich M. M. Bogush V. G. Sokolova O. S. Sevastyanov V. I. et al. 2009 Three-dimensional scaffold made from recombinant spider silk protein for tissue engineering.Dokl Biochem Biophys, 426 127 130.
(2006). Use of spider silk fibres as an innovative material in a biocompatible artificial nerve conduit. J Cell Mol Med, 10(3), 770-777. Allmeling C. Jokuszies A. Reimers K. Kall S. Vogt P. M.
Ando Y. Okano R. Nishida K. Miyata S. Fukade E. 1980Piezoelectric and related properties of hydrated silk fibroin. Rep Prog Polymer Physics Japan, 23 775 778.
Askarieh G. Hedhammar M. Nordling K. Saenz A. Casals C. Rising A. Johansson J. Knight S. 2010 Self-assembly of spider silk proteins is controlled by a pH-sensitive relay. , 465(7295), 236 238.
Ayoub N. A. Garb J. E. Tinghitella R. M. Collin M. A. Hayashi C. Y. 2007 Blueprint for a high-performance biomaterial: full-length spider dragline silk genes., 2, e514.
Bini E. Foo C. W. Huang J. Karageorgiou V. Kitchel B. Kaplan D. L. 2006 RGD-functionalized bioengineered spider dragline silk biomaterial., 7(11), 3139 45.
Blasingame E. Tuton-Blasingame T. Larkin L. Falick A. M. Zhao L. Fong J. Vaidyanathan V. Visperas A. Geurts P. Xu X. La Mattina C. Vierra C. 2009 Pyriform spidroin 1, a novel member of the silk gene family that anchors dragline silk fibers in attachment discs of the black widow spider, Latrodectus hesperus.(42), 29097-29108.
Brooks A. E. Nelson S. R. Jones J. A. Koenig C. Hinman M. Stricker S. Lewis R. 2008 Distinct contributions of model MaSp1 and MaSp2 like peptides to the mechanical properties of synthetic major ampullate silk fibers as revealed in silico. Nanotechnol Sci Appl, 1 9 16.
Casem M. L. Turner D. Houchin K. 1999 Protein and amino acid composition of silks from the cob weaver, Latrodectus hesperus (black widow).(2-3), 103 8.
Casem M. L. Tran L. P. Moore A. M. 2002 Ultrastructure of the major ampullate gland of the black widow spider, Latrodectus hesperus. (6), 427 EOF 436 EOF.
Chen X. Knight D. P. Vollrath F. 2002 Rheological characterization of Nephila spidroin solution., 3(4), 644 8.
Craig C. L. Riekel C. Herberstein M. E. Weber R. S. Kaplan D. Pierce N. E. 2000 Evidence for diet effects on the composition of silk proteins produced by spiders.(12), 1904 13.
Dicko C. Vollrath F. Kenney J. M. 2004 Spider silk protein refolding is controlled by changing pH., 5(3), 704 10.
Du N. Liu X. Y. Narayanan J. Li L. Lim M. L. Li D. 2006 Design of superior spider silk: from nanostructure to mechanical properties. (12), 4528-4535.
Fahnestock S. R. Bedzyk L. A. 1997 Production of synthetic spider dragline silk protein in Pichia pastoris.(1), 33 9.
Foelix R. 1996 Biology of spiders. New York: Oxford University Press.
Gellynck K. Verdonk P. C. Van Nimmen E. Almqvist K. F. Gheysens T. Schoukens G. Van Langenhove L. Kiekens P. Mertens J. Verbruggen G. 2008 Silkworm and spider silk scaffolds for chondrocyte support. (11), 3399-3409.
Gosline J. M. De Mont M. E. Denny M. W. 1986 The structure and properties of spider silk. , 10 31 43.
Gosline J. M. Guerette P. A. Ortlepp C. S. Savage K. N. 1999 The mechanical design of spider silks: from fibroin sequence to mechanical function. ., 202(Pt 23), 3295-3303.
Geurts P. Zhao L. Hsia Y. Gnesa E. Tang S. Jeffery F. La Mattina C. Franz A. Larkin L. Vierra C. Synthetic spider silk fibers spun from Pyriform Spidroin. , 11(12), 2a glue silk protein discovered in orb-weaving spider attachment discs 3495 3503.
Guerette P. A. Ginzinger D. G. Weber B. H. Gosline J. M. 1996 Silk properties determined by gland-specific expression of a spider fibroin gene family. , 272(5258), 112 115.
Hagn F. Eisoldt L. Hardy J. G. Vendrely C. Coles M. Scheibel T. Kessler H. 2010 A conserved spider silk domain acts as a molecular switch that controls fibre assembly. , 465(7295), 239 242.
Hayashi C. Y. Blackledge T. A. Lewis R. V. 2004 Molecular and mechanical characterization of aciniform silk: uniformity of iterated sequence modules in a novel member of the spider silk fibroin gene family. (10), 1950-1959.
Hedhammar M. Bramfeldt H. Baris T. Widhe M. Askarieh G. Nordling K. Aulock S. Johansson J. 2010 Sterilized recombinant spider silk fibers of low pyrogenicity. , 11(4), 953 959.
Hinman M. B. Lewis R. V. 1992 Isolation of a clone encoding a second dragline silk fibroin. Nephila clavipes dragline silk is a two-protein fiber.(27), 19320 4.
Hu X. Lawrence B. Kohler K. Falick A. M. Moore A. M. Mc Mullen E. Jones P. Vierra C. 2005 Araneoid egg case silk: a fibroin with novel ensemble repeat units from the black widow spider, Latrodectus hesperus., 44(30), 10020 7.
Hu X. Vasanthavada K. Kohler K. Mc Nary S. Moore A. M. Vierra C. A. 2006a Molecular mechanisms of spider silk. (17), 1986 1999.
Hu X. Kohler K. Falick A. M. Moore A. M. Jones P. R. Vierra C. 2006b Spider egg case core fibers: trimeric complexes assembled from TuSp1, ECP-1, and ECP-2., 45(11), 3506 16.
Hu X. Yuan J. Wang X. Vasanthavada K. Falick A. M. Jones P. R. La Mattina C. Vierra C. 2007 Analysis of aqueous glue coating proteins on the silk fibers of the cob weaver, Latrodectus hesperus., 46(11), 3294 303.
Huemmerich D. Helsen C. W. Quedzuweit S. Oschmann J. Rudolph R. Scheibel T. 2004 Primary structure elements of spider dragline silks and their contribution to protein solubility., 43(42), 13604 12.
Jeffery F. La Mattina C. Tuton-Blasingame T. Hsia Y. Gnesa E. Zhao L. Franz A. Vierra C. 2011Microdissection of black widow spider silk-producing glands. (47).
Knight D. P. Knight M. M. Vollrath F. 2000 Beta transition and stress-induced phase separation in the spinning of spider dragline silk.(3), 205 10.
Knight D. P. Vollrath F. 2001 Changes in element composition along the spinning duct in a Nephila spider. , 88(4), 179 182.
Lammel A. Schwab M. Hofer M. Winter G. Scheibel T. 2011 Recombinant spider silk particles as drug delivery vehicles. , 32(8), 2233 2240.
Lawrence B. A. Vierra C. A. Moore A. M. 2004 Molecular and mechanical properties of major ampullate silk of the black widow spider, Latrodectus hesperus., 5(3), 689 95.
Lazaris A. Arcidiacono S. Huang Y. Zhou J. F. Duguay F. Chretien N. Welsch E. Soares J. Karatzas C. 2002 Spider silk fibers spun from soluble recombinant silk produced in mammalian cells. , 295(5554), 472 476.
Lefevre T. Boudreault S. Cloutier C. Pezolet M. 2008 Conformational and orientational transformation of silk proteins in the major ampullate gland of Nephila clavipes spiders. , 9(9), 2399 2407.
Lefevre T. Boudreault S. Cloutier C. Pezolet M. 2011 Diversity of molecular transformations involved in the formation of spider silks. (1), 238 253.
Lewis R. V. 2006 Spider silk: ancient ideas for new biomaterials.(9), 3762 74.
Lin L. H. Edmonds D. T. Vollrath F. 1995 Structural engineering of an orb-spider’s web. , 373 146 148.
Lin Z. Huang W. Zhang J. Fan J. S. Yang D. 2009 Solution structure of eggcase silk protein and its implications for silk fiber formation. (22), 8906-8911.
Liivak O. Flores A. Lewis L. Jelinski L. W. 1997 Conformation of the polyalanine repeats in minor ampullate gland silk of the spider Nephila clavipes. , 30 7127 7130.
Lombardi S. Kaplan D. L. 1990 The Amino Acid Composition of Major Ampullate Gland Silk (Dragline) of Nephila clavipes (Araneae, Tetragnathidae). J. Arachnol., 18 297 306.
Michal C. A. Simmons A. H. Chew B. G. Zax D. B. Jelinski L. W. 1996 Presence of phosphorus in Nephila clavipes dragline silk.(1), 489-493.
Nova A. Keten S. Pugno N. M. Redaelli A. Buehler M. J. 2010 Molecular and nanostructural mechanisms of deformation, strength and toughness of spider silk fibrils. (7), 2626 2634.
Ortiz R. Cespedes W. Nieves L. Robles I. V. Plazaola A. File S. et al. 2000 Small ampullate glands of Nephila clavipes.(2), 114 9.
Pouchkina N. N. Stanchev B. S. Mc Queen-Mason S. J. 2003 From EST sequence to spider silk spinning: identification and molecular characterisation of Nephila senegalensis major ampullate gland peroxidase NsPox.(2), 229 38.
Scheller J. Guhrs K. H. Grosse F. Conrad U. 2001 Production of spider silk proteins in tobacco and potato.(6), 573 73-577.
Schmidt M. Romer L. Strehle M. Scheibel T. 2007Conquering isoleucine auxotrophy of BLR(DE3) to recombinantly produce spider silk proteins in minimal media. Biotechnol Lett, 29(11), 1741-1744.
Shao Z. Vollrath F. Yang Y. Thogersen H. 2003 Structure and Behavior of Regenerated Spider Silk. , 36 1157 1161.
Simmons A. H. Michal C. A. Jelinski L. W. 1996 Molecular orientation and two-component nature of the crystalline fraction of spider dragline silk. , 271(5245), 84-87.
Sponner A. Unger E. Grosse F. Weisshart K. 2005 Differential polymerization of the two main protein components of dragline silk during fibre spinning.(10), 772 5.
Sponner A. Vater W. Monajembashi S. Unger E. Grosse F. Weisshart K. 2007 Composition and hierarchical organisation of a spider silk., 2(10), e998.
Stark M. Grip S. Rising A. Hedhammar M. Engstrom W. Hjalm G. et al. 2007 Macroscopic fibers self-assembled from recombinant miniature spider silk proteins., 8(5), 1695 701.
Szela S. Avtges P. Valluzzi R. Winkler S. Wilson D. Kirschner D. Kaplan D. 2000 Reduction-oxidation control of beta-sheet assembly in genetically engineered silk., 1(4), 534 42.
Teule F. Cooper A. R. Furin W. A. Bittencourt D. Rech E. L. Brooks A. Lewis R. 2009 A protocol for the production of recombinant spider silk-like proteins for artificial fiber spinning.(3), 341 55.
Tso I. M. Wu H. C. Hwang I. R. 2005 Giant wood spider Nephila pilipes alters silk protein in response to prey variation.(Pt 6), 1053 61.
Vasanthavada K. Hu X. Falick A. M. La Mattina C. Moore A. M. Jones P. R. Yee R. Reza R. Tuton T. Vierra C. 2007 Aciniform spidroin, a constituent of egg case sacs and wrapping silk fibers from the black widow spider Latrodectus hesperus.(48), 35088 97.
Vollrath F. Wen Hu. X. Knight D. P. 1998 Silk production in a spider involves acid bath treatment. Proc. R. Soc. B, 263 817 820.
Vollrath F. Barth P. Basedow A. Engstrom W. List H. 2002 Local tolerance to spider silks and protein polymers in vivo.(4), 229 34.
Winkler S. Szela S. Avtges P. Valluzzi R. Kirschner D. A. Kaplan D. 1999 Designing recombinant spider silk proteins to control assembly.(2-3), 265 70.
Winkler S. Wilson D. Kaplan D. L. 2000 Controlling beta-sheet assembly in genetically engineered silk by enzymatic phosphorylation/dephosphorylation., 39(41), 12739 46.
Xia X. X. Qian Z. G. Ki C. S. Park Y. H. Kaplan D. L. Lee S. Y. 2010 Native-sized recombinant spider silk protein produced in metabolically engineered Escherichia coli results in a strong fiber. (32), 14059 14063.
Xu M. Lewis R. V. 1990 Structure of a protein superfiber: Spider Dragline Silk.Proc. Natl. Acad. Sci., 87 7120 7124.
Xu H. T. Fan B. L. Yu S. Y. Huang Y. H. Zhao Z. H. Lian Z. X. Dai Y. P. Wang L. L. Liu Z. L. Fei J. Li N. 2007 Construct synthetic gene encoding artificial spider dragline silk protein and its expression in milk of transgenic mice.Anim Biotechnol, 1 12.
Yang J. Barr L. A. Fahnestock S. R. Liu Z. B. 2005 High yield recombinant silk-like protein production in transgenic plants through protein targeting. (3), 313 324.
Zhao A. Zhao T. Sima Y. Zhang Y. Nakagaki K. Miao Y. et al. 2005 Unique molecular architecture of egg case silk protein in a spider, Nephila clavata. (5), 593 604.
Zhao A. C. Zhao T. F. Nakagaki K. Zhang Y. S. Sima Y. H. Miao Y. G. Kajiura Z. Nagata Y. Takadera M. Nakagaki M. 2006 Novel molecular and mechanical properties of egg case silk from wasp spider, Argiope bruennichi., 45(10), 3348 56.